Dental Materials Journal 2015; 34(2): 211–218
Evaluation of glass transition temperature and dynamic mechanical properties of autopolymerized hard direct denture reline resins Kazuma TAKASE1, Ikuya WATANABE2, Tadafumi KUROGI1 and Hiroshi MURATA1 Department of Prosthetic Dentistry, Graduate School of Biomedical Sciences, Nagasaki University, 1-7-1 Sakamoto, Nagasaki, 852-8588, Japan Department of Dental and Biomedical Materials Science, Graduate School of Biomedical Sciences, Nagasaki University, 1-7-1 Sakamoto, Nagasaki, 852-8588, Japan Corresponding author, Hiroshi MURATA; E-mail: [email protected]
This study assessed methods for evaluation of glass transition temperature (Tg) of autopolymerized hard direct denture reline resins using dynamic mechanical analysis and differential scanning calorimetry in addition to the dynamic mechanical properties. The Tg values of 3 different reline resins were determined using a dynamic viscoelastometer and differential scanning calorimeter, and rheological parameters were also determined. Although all materials exhibited higher storage modulus and loss modulus values, and a lower loss tangent at 37˚C with a higher frequency, the frequency dependence was not large. Tg values obtained by dynamic mechanical analysis were higher than those by differential scanning calorimetry and higher frequency led to higher Tg, while more stable Tg values were also obtained by that method. These results suggest that dynamic mechanical analysis is more advantageous for characterization of autopolymerized hard direct denture reline resins than differential scanning calorimetry. Keywords: Reline resin, Glass transition temperature, Dynamic mechanical analysis, Differential scanning calorimetry
INTRODUCTION Autopolymerized hard direct denture reline resins are widely used to provide accurate adaptation between the denture intaglio surface of complete and removable partial dentures and denture foundation areas1) changed due to residual ridge resorption2). A procedure of reline improves the stability and retention of ill-fitting dentures. Although an indirect (laboratoryprocessed reline system) method has also been used, the direct method (chair-side reline system) using autopolymerized hard direct denture reline resins is applied in nearly all clinical situations, because sending the denture to a dental laboratory is not required and the procedure is easier than that of an indirect method3). In general, the powder component used in autopolymerized reline resins is based on poly(methyl methacrylate), poly(ethyl methacrylate), or poly(methyl methacrylate/ethyl methacrylate), while the liquid component consists of a monofunctional methacrylate monomer, polyfunctional monomer (cross-linking agent), or those in combination4). A chemically activated accelerator such as tertiary amine is also added to the liquid to produce the autopolymerization reaction5). The differences in composition and structure among the available materials have great influence on mechanical properties3,6-8), manipulation3), durability3), water absorption and solubility of the liquid components3,6,7,9), bond strength to denture base resins10-12) and exothermic reactions during polymerization13-15) with mechanical properties especially important for the lifetime of dentures with denture reline resins. The properties of denture reline resins have been determined by findings obtained in a 3-point bending test6,7), Knoop hardness test12) and dynamic mechanical test3,8,15,16). Furthermore, Received Oct 2, 2014: Accepted Nov 11, 2014 doi:10.4012/dmj.2014-277 JOI JST.JSTAGE/dmj/2014-277
glass transition temperature (Tg) has great significance from a practical point of view, as polymers generally exhibit a large variation of mechanical properties with temperature. At sufficiently low temperature, amorphous polymers, which are widely used in dental materials, behave as rigid solids, and when the temperature is increased they behave as flexible solids, rubber, or viscous liquid5). The transition from hard brittle to soft flexible material is shown by Tg17). Large polymer chains can move freely at Tg18) though such movement is dependent on the molecular structure, as well as degree of cross-linking and branching5). Thermal properties including the Tg values of materials used for dentures have primarily been investigated by dynamic mechanical analysis (DMA)3,8,15,18-20) and differential scanning calorimetry (DSC)18,21,22). Dynamic mechanical analysis is one of the most useful techniques available for evaluating the mechanical properties of materials with cyclic applications of stress and temperature. In a dynamic mechanical test, sinusoidal tensile strain is applied to one end of a specimen and stress response is measured at the other end. When the specimen is a perfectly elastic solid, the strain is in exact phase with the applied stress, while the strain is 90° out of phase in a perfectly viscous liquid. For a viscoelastic material, the strain is somewhere in between (π/2>δ>0)16,23). Generally, 3 rheological parameters, storage modulus (E'), loss modulus (E" ), and loss tangent (tan δ), are determined for evaluation of the dynamic mechanical properties of the tested material. E' shows elastic deformation under stress and corresponds to completely recoverable energy, while E" shows viscous deformation and corresponds to energy loss from heat dissipation, and tan δ shows the relative contributions of the elastic and viscous
Dent Mater J 2015; 34(2): 211–218
components, that is, a measure of the ratio of energy lost to energy stored during cyclic deformation. This parameter reveals overall material behavior16,23). The Tg value of a tested material can be determined from a graphic representation of tan δ or E" 3,20,24-26). Differential scanning calorimetry is essentially a thermal analysis technique used to measure temperatures and heat flow related to the thermal transition of materials24,27,28). When using a differential scanning calorimeter, 2 pans are connected to the heater. The specimen is placed into 1 and the remaining pan is used as a reference. Heat flow to each pan is monitored, and the differential between the specimen and the reference is determined, which provides variations in heat capacity with temperature of the tested material18). The Tg value can be determined as a downward step in heat flow using a differential scanning calorimetry trace18). A previous study evaluated Tg of mouthguard materials by both dynamic mechanical analysis and differential scanning calorimetry28), and found no significant differences among various commercial materials for mean Tg values. On the other hand, differences between the Tg values obtained from dynamic mechanical analysis and differential scanning calorimetry were noted for all of the tested materials. Those findings will indicate that the Tg value of other dental materials such as autopolymerized hard direct denture reline resins may vary based on the test method used. Furthermore, for a dynamic mechanical test, it is necessary to evaluate the influence of frequency on calculated Tg values, because rheological parameters such as E', E", and tan δ vary based on the frequency applied to the materials25,29). However, there is scant information regarding Tg evaluation methods for use with autopolymerized hard direct denture reline resins. The purpose of the present study was to assess evaluation methods for Tg values of autopolymerized hard direct denture reline resins obtained using dynamic mechanical analysis and differential scanning calorimetry. In addition, the dynamic mechanical
properties of the tested reline resins and influence of frequency on those properties were also determined. Prior to performing the study, we speculated that differences in the obtained Tg values would be found between these 2 methods and that frequency applied in the dynamic mechanical test would have an influence on determination of Tg.
MATERIALS AND METHODS Table 1 shows the autopolymerized hard direct denture reline resins used in the present study, together with manufacturer and general composition. The glass transition temperatures (Tg) values of the tested materials were determined by means of dynamic mechanical analysis and differential scanning calorimetry. Dynamic mechanical analysis (DMA) Dynamic mechanical analysis of the materials was performed using an automatic dynamic viscoelastometer (Rheovibron DDV-25FP, A&D Co. Ltd., Tokyo, Japan) based on the principle of nonresonance forced vibration3,16). Five samples of each material were prepared in the form of rectangular blocks (25.0×7.0×2.0 mm) using a metal mold. Tests for temperature dependence of the dynamic mechanical properties were conducted at 0.1, 0.2, 1, 5 and 10 Hz over a temperature range of 25–200˚C at 2 h after sample preparation to determine the glass transition temperature (Tg) of the tested material. The ends of the samples were held with a span of 15 mm and strain amounting to 0.05% was added16). The rheological parameters tensile storage modulus (E’), tensile loss modulus (E”), and loss tangent (tan δ) were then calculated using the following the equations: E*=E'+iE" E'=|E*|cosδ E"=|E*|sinδ tan δ=E"/E'
Table 1 Autopolymerized hard direct denture reline resins tested Material
Powder: 00076A, Liquid: 00026A
Kuraray Noritake Dental Inc., Tokyo, Japan
Fluorinated monomer, Other methacrylate monomer
Powder: 1205-188, Liquid: 1204-150
The Harry J. Bosworth Co, Skokie, Il, USA
Iso-butyl methacrylate Dibutyl phthalate
Powder: 1211021, Liquid: 1106011
GC Corp., Tokyo, Japan
Methyl methacrylate Dibutyl sebacate
*Composition as given by manufacturers and reference 4)
Dent Mater J 2015; 34(2): 211–218
Where E* is the complex dynamic tensile modulus, i √1 and δ the phase angle between stress and strain. Tg was defined as the temperature corresponding to the maximum of the tan δ peak position3,8,20,26). Differential scanning calorimetry (DSC) Differential scanning calorimetry was conducted using a differential scanning calorimeter (DSC-60, Shimadzu Corp., Kyoto, Japan) to determine Tg. Each specimen was placed into an aluminum pan and the tests were performed under a nitrogen purge with a flow rate of 50 mL/min. The scan speed for thermal heating was 2˚C/ min and the temperature range was from 25–200˚C. The heat flow of each material was plotted against the temperature (time) (DSC curve). The Tg values of the test materials were determined according to JIS (Japanese Industrial Standards) K 7121:198730) with 5 tests conducted for each material. Statistical analyses Five tests were carried out for each measurement and material. Comparisons of Tg values obtained by dynamic mechanical analysis at various frequencies and differential scanning calorimetry were subjected to oneway analysis of variance (ANOVA), and the mean values were compared using Tukey’s method at a 5% level of significance. The above statistical analyses of E′, E″, and tan δ values at 1 Hz and 37˚C were also conducted to determine differences among the materials. A t-test was used to determine whether statistically significant differences existed between E′ and E″ for 1 Hz and 37˚C. For all statistical analyses, a statistical analysis software (SPSS Statistics version 17.0, SPSS Inc., Chicago, IL, USA) was used.
RESULTS There were variations in the obtained storage modulus (E′), loss modulus (E″), and loss tangent (tan δ) values with changes in temperature for the 3 autopolymerized hard direct denture reline resins at various frequencies (Figs. 1–3). The E′ values for Kurarebase, New Truliner, and Rebaron were greatly decreased at approximately 50˚C, 60˚C, and 40˚C, respectively, while their E″ values were also greatly decreased at ranges of approximately 60–70˚C, 70–80˚C, and 90–100˚C, respectively. Both the E′ and E″ values of the 3 materials tended to be higher at higher frequencies. As shown in the figures, the curves of E′ and E″ became shifted to the right side with increasing frequency. Furthermore, the tan δ values for the 3 materials were increased with increasing temperature until the maximum level was reached, then decreased. The peak of tan δ, namely glass transition temperature (Tg), for Kurarebase at 0.1, 0.2, 1, 5, and 10 Hz was observed at approximately 70˚C, 70˚C, 73˚C, 77˚C, 85˚C, and 89˚C, respectively, while those for New Truliner were observed at approximately 62˚C, 64˚C, 68˚C, 72˚C, 79˚C, and 84˚C, respectively, and for Rebaron were observed at approximately 86˚C, 87˚C, 89˚C, 92˚C, and 99˚C, respectively. The peak of tan δ (Tg)
Variations in storage modulus (E′ ), loss modulus (E″ ), and loss tangent (tan δ) values with temperature for Kurarebase at various frequencies.
of the materials demonstrated a tendency to shift to the right side, that is to higher temperature, with increasing frequency, as shown in the figures. Figure 4 shows variations in the E′, E″ and tan δ values with different frequencies for the 3 tested materials at 37˚C. The values for E′ and E″ increased with increasing frequency, whereas tan δ tended to decrease with increased frequency. Figure 5 shows the E′, E″, and tan δ values for the 3 tested materials at 1 Hz and 37˚C. The values of E′ were significantly higher (p